Enhancing the Creep Resistance of Sn-9 . 0 Zn-0 . 5 Al Lead-Free Solder Alloy by Small Additions of Sb Element

The creep phenomenon is considered as one of the most important deformation mechanisms under working conditions. The present study has examined the microstructure and creep properties of Sn-9.0Zn-0.5Al solder alloy after adding a small amount of Antimony (Sb). Nominal compositions of Sb additions were chosen to be 0, 0.5, 1.0, and 1.5 wt.%. The minimum strain rate was reduced for the Sb containing solder alloy. The stress exponents, n, were found to be around 3.7 for all soldiers at 130 ̊C. The stress exponent increases as the temperature drops from 100 ̊C to 50 ̊C, except for the 1.0% Sb alloy, where n 5.3 6.1 at all the temperature range (T = 50 ̊C, 100 ̊C and 130 ̊C). The results reveal that the Sb-containing solder alloys have better creep resistance with greater ductility than the Sb-free alloy due to solid solution strengthening, and intermetallic compound SnSb particle hardening.


Introduction
Sn-9Zn eutectic alloy has been considered as one of the candidate that can be replaced the Sn-37Pb solder without increase of the operating temperature.Apart from its favorable melting temperature of solder alloys, Sn-9Zn alloy has better mechanical properties than the conventional Sn-Pb solders [1] [2] [3], and a lower cost than other Lead-free solders alloys [4] [5].Whenever such alloys are used for many electronic applications, they are subjected to yield many prob-E.A. Eid et al.DOI: 10.4236/eng.2018.101003 22 Engineering lems, such as, the tendency of oxidation and poor wetting ability [5].Therefore, the researchers tried to add a third element to overcome the shortfalls of Sn-9Zn alloy.Consequently, it is necessary to understand how the oxidation resistance, wettability, corrosion, melting temperature, and mechanical properties are changed because of the third alloying element addition.
For example, the third element suggesting adding to Sn-9Zn eutectic alloy are Ag [4] [5], Bi [6] [7], In [8], Al [9] [10] and Ce/La [11] [12].For instance, McCormack and Jin [8] found that small additions of 5% In can improve the ductility of Sn-Zn base solders.It was found also that the wetting characteristics are improved when Ag is added [5] [13].Moreover, Kim et al. [6] found that with increasing of additional Bi content, the melting temperature decreased from 198.4˚C to 186.1˚C.However, the alloys with a high Bi content need to be controlled because of the brittle nature of Bi and the strong tendency for segregation [6] [14].Chen and Li [15] reported that adding Recently, our group reveled that adding a small amount of Sb to the Sn-9Zn-0.5Alsystem refined the bulky needles of Zn as well as β-Sn matrix.In addition, it improved strengthen by solid solution hardening mechanism [3].In same time, it is known that under the conventional operating conditions, the solder joints are exposed to aggressive thermo-mechanical cycling (TMC), with imposed shear strain under high homologous temperatures T H (T H = T/T m ) [20].
Therefore, the creep phenomenon is considered as the most important deformation mechanism under working conditions.Additionally, the literatures have rare studies about the effect of Sb as an alloying element on the creep properties of Sn-Zn-Al solder system.Therefore, the present study focused on the effect of Sb alloying element on the reliability characteristics of Sn-  air-cooled to the room temperature.The air-cooling is equivalent to that adopted in the particle reflow process in industry.The cooling rate estimated by using a thermocouple placed in the center of solder.The ingots were cold drawn to wire samples of 8 × 10 −4 m in diameter and 5 × 10 −2 m length.To obtain stabilized microstructures, the alloy samples were aged at 130˚C for 3 hours, and then slow cooled to room temperature.The as-solidified microstructure of the solders was investigated using X-ray diffraction (Philips Analytical X-Ray PW3710) and Nikon optical microscope, where the grain sizes was estimated using a linear intercept technique.Tensile creep tests were performed using homemade instrument, the resulting strain recorded as a function of time under constant applied stresses ranging from 15.6 to 29.3 MPa at constant temperatures of 50˚C, 100˚C, and 130˚C.The accuracy of temperature measurement is of the order 1˚C.Strain measurements were done with an accuracy of 1 × 10 −2 mm.

As-Solidified Microstructure
Optical micrographs of specimens with varying x % Sb (x = 0, 0.5, 1.0 and 1.5) contents are presented in Figure 1.The bright-gray area and dark-gray area in Figure 1 denotes the primary β-Sn phase and eutectic (Sn + Zn) networks, respectively.This result is consistent with binary-phase diagram of Sn-Zn, which shows a typical binary-eutectic phase diagram with no intermetallic compounds and limited solubility of the two elements in each phase [9].Much coarser primary β-Sn grains can be found only in the Sn-9.0Zn-0.5Al(SZA905) alloy as shown in Figure 1(a).In addition, the microstructure of the Sb-free alloy is not uniform.The formation of fully individualized and spheroid grains occurred during solidification at cooling rate of 10˚C/s.Similar microstructures are observed in some Lead-free solder alloys at earlier solidification rates of 12˚C/s and 10˚C/s in studies [17]., at a temperature above 234.8˚C, the presence of Sb in Sn-Zn eutectic seems to simulate the formation of SnSb intermetallic compound (IMC) in molten solder.The SnSb phase is a stable phase and exists in the form of small particles that are finally dispersed in the matrix phase [23], which offers preferred sites for nucleation, resulting in grain refining and uniform microstructure as reported in our previous work [3].
The XRD micrographs for Sn-9.0Zn-0.5Al-xSb% (x = 0.0, 0.5, 1.0 and 1.5 wt %) lead free solder alloys are depicted in Figure 2. Presence of (200), (101), (211) and (321) peaks at 2θ values of 31.2˚,33.6˚, 45.3˚, and 64.8˚ respectively, confirm the formation of body centered tetragonal (BCT) crystal structure of β-Sn for all investigated alloys.Meanwhile, the XRD patterns of Sb-containing alloys exhibited obviously decrement in intensity of (002) and (100) of Zn crystallographic textures.The latter observation is detail discussed in our pervious article, which confirmed hypoeutectic composition is formed [3].On other hand, no peaks of Al element were observed while SbSn IMC phase was detected as a small peak for 1.5 wt % Sb-content solder.That indicated the Sb atoms have successfully replaced the corresponding position of Sn atoms at BCT lattice sites for SZA-1.5 Sb lead free solder alloys [24].and time (t) are normalized with respect to the rupture strain (ε f ) and rupture Engineering time (τ f ), respectively.At 50˚C, the fraction of the steady-state creep strain increased against the rupture strain (ε s /ε f ) because of Sb additions, and that effect was maximized at 1.0% Sb.Whereas increasing the temperature from 50˚C to 100˚C resulted in decreasing the fraction (ε s /ε f ) for the 1.0% Sb alloy and enhanced the creep resistance (i.e., lowered) which is associated with the dissolution of Sb rich β-Sn phase in the matrix [25].

Stress Dependence of Minimum Creep Rate
The minimum strain rate was measured as a function of stress and temperature from the linear portions of the creep curves for the four solder compositions.
Stress exponents, n, were calculated from the power-law creep expression, min creep resistance at all the temperature range, while the Sb-free alloy showed the worst one.The major anomaly in the data is in the temperature dependence of stress exponent.At 130˚C, n values were usually around 3.7 for all solder alloys except for 1.0% Sb specimens, which showed high n value of 5.3.The values of stress exponents for all solder alloys increase rapidly as the temperature decreases from 100˚C to 50˚C, except the 1.0% Sb alloy which showed almost identical stress exponent of 5.3 -6.1 at 50˚C and 100˚C, a range of significant technological interest.
It appears that the amount of Sb dissolved in the solution-strengthened matrix phase varies with different Sn-9.0Zn-0.5Alsolder systems.It is assumed that the stable characteristics of mechanical properties resulted in the strengthening effect of the solute concentration [2] [18] [22].Sb element has higher affinity to the constituent element of Sn in the Sn-Zn-Al-Sb quaternary system.It will reduce the activity of Sn by forming solid solution hardening and particle hardening of Sb rich β-Sn phase, resulting in refinement of the grain size, and thus improved the creep resistance as reported by Chen et al. [15].However, the change in creep behavior with temperature is consistent with the observations of Song and Morris [21], Breen and Weertman [26], Suh et al. [27], and Poirie [28].They noted significant changes in creep behavior of Sn-rich solders at about 100˚C.The data presented in Figure 7 show the range of stress exponent (n ~ 3.7 -6.1) is comparable to that of Sn and Sn-rich solders, corresponding to climb-controlled creep (n~4 -5) reported by Breen and Weertman [26] and Song and Morris [21].Dislocation climb-controlled creep is generally described by a power law equation of the form [22] [31]: where A is a constant, R is the gas constant, n is the stress exponent and Q is the activation energy.The apparent activation energy, Q, of the creep process was determined from Arrhenius plot ( log ε versus 1/T), as shown in Figure 8, the values of, Q, for the process estimated to be 40 ± 2 kJ/mole for Sb-containing solders and Sb-free solder alloy as depicted in Figure 9, which are comparable to that reported for the pipe diffusion controlled climb of tin (43 -46 kJ/mole) [29]

Conclusions
The main conclusions to be drawn from this study may be summarized as follows: 1) The originally coarse β-Sn grains in the microstructure of Sn-9.0Zn-0.5Alsolder alloy were refined and become uniform after Sb additions due to the solute concentration and the finally dispersed SnSb particles in the matrix, which offer preferred sites for nucleation during solidification.
2) The Sb-containing solders have better creep resistance and greater ductility than the Sn-9.0Zn-0.5Alsolder alloy, and the effect was usually found to reduce and increase rupture time τ f .

Figures 3 (Figure 2 .
Figures 3(a)-(c) show the results of creep test obtained for Sn-9.0Zn-0.5Al-xSb(x = 0.0%, 0.5%, 1.0%, and 1.5%) solder alloys.The samples were investigated at temperatures of 50˚C, 100˚C, and 130˚C under different constant stresses (15.6 -29.3 MPa).The trend in the creep curves at all levels of applied stresses and temperatures suggests a rapid transition from a little primary creep regime, to an extended period of constant strain rate with tertiary creep regime.This transition

Figure 3 .Figure 4 .
Figure 3.Comparison of the creep behavior of the four solder alloys under different stress at (a) 50˚C, (b) 100˚C and (c) 130˚C.